The Effect of Flat Panel Reflectors on Photovoltaic Energy
Harvesting in Wireless Sensor Nodes under Low
Sapavat Deepa & Ramavath Shankar Naik
*Assistant Professor with the DepartmentElectronics& Communication Engineering.at SLC College
**Assistant Professor with the Department of Electrical &Electronic Engineering at SLC College
The electric double layer is known to affect thin-film lubrication. Other researchers have shown that tribocharging affects the breaking torque in a metal shaft-oil-lip seal system and that an external electric field may be employed to control this phenomenon. One main issue in all these studies is the characterization of the charging state of the bodies in contact. This is quite a difficult challenge when the contact occurs between two insulating materials. The ultimate aim of this paper is to validate an experimental procedure appropriate for ensuring the reproducibility of the tribocharging conditions in sliding contacts between polymeric materials. The experiments were performed with samples of polystyrene and polyvinyl chloride. Surface potential measurements were done to evaluate the tribocharging effects. The experiments pointed out that the amount of charge accumulated on the sliding bodies depends on the external force applied to the contact and the number of
tribocharging cycles (i.e., back-and-forth relative motions). However, this charge is nonuniformly distributed on the surface of the samples. This means that it will be difficult to use the tribocharging effect for controlling the charging state and, hence, the lubrication of the contact between two insulating bodies
INTRODUCTION Polymers are more and
braking torque . The reported experimental data reveal the influence of tribocharging of synthetic motor base oils blended with different additives friction modifiers (FM) and antiwear agents (AW). The DC electric field is used to compensate for the natural electric field generated by the net charge of mobile ions and molecules in the zone between rotating metal shaft and the lip of the seal . Electrical charges generation occurring during contact and friction of insulating materials has been studied for a long time , . Various test methodologies have been proposed for this so-called “triboelectrification” effect , , which strongly depends on load, on sliding speed and on ambient conditions -, and affects friction and wear -. It is possible to control the triboelectrification of rubbing elements by using appropriate materials, according to their position in a triboelectric series . Most of these triboelectrification
studies were performed with devices
characterized by non-conformal contacts. In such devices, the area of contact between the surfaces is very small; as a result, the contact pressure is high and the wear of the surfaces is significant even under low load. The respective experimental benches typically provide uni-directional relative movement of the bodies in contact: a pin and a rotating disk or two rolling
rings. The rotational movement is accompanied by charge generation due to the continuous friction between the two bodies. Fewer studies were made on the tribocharging phenomena associated to conformal contacts, where the surface of the contact area is comparable with the size of the bodies involved . The benches described in the literature were typically making use of crank – shaft mechanisms to provide back-and-forth motion between the bodies in contact , . In the present paper, the sliding contact occurs between two plate-type samples, one fixed and the other attached to a bi-directional belt
conveyor. Triboelectrification has been
conditions in sliding contacts between polymeric materials.
Fig. 1. Photograph of the tribocharging system.
Fig. 2. Schematic representation of the experimental procedure: the bidirectional belt conveyor moves the
sample A back-and-forth with respect with the central axis of sample B (two tribocharging cycles), then carries it under the capacitive probe of the electrostatic voltmeter
(the axis of the probe is located in the vertical plane defined by the central transversal axis of the sample A) .
II. MATERIALS AND METHOD
poly-vinyl-chloride (PVC). The samples were cut in
two sizes: A (50 mm x 183 mm) and B (100 mm
x 15 mm). The samples Aare fixed on a
grounded metallic electrode (200 mm x 200 mm), placed on a carrier attached to a conveyor belt (Fig. 1). A reversible DC motor entrains the conveyor and the carrier at a fixed speed of 100
mm/s. The samples B are attached to a
tribocharging device that can impose a load of 1 N or 2 N on the surface of contact between the
two samples (size: 50 mm x 15 mm; the long
axis of sample B is parallel to the short axis of
sample A). The device is carried by an arch-type
support, as shown in Fig. 1. In this way, the
sample B has a fixed position in horizontal
plane, and can move only in vertical direction,
so that to be in free contact with the sample A.
The latter can move back-and-forth for a distance of 150 mm, symmetrical with respect to
the central axis of the sample B (Fig. 2).
Fig. 3. Schematic representation of the 2D zone scanned by the probe of the electrostatic voltmeter at the
surface of the A-type sample
A tribo-charging cycle typically consisted in such a back-and-forth motion. Two cycles were found to be enough for the accumulated charge to be detected by the measurement of the
electrical potential at the surface of sample A. In
a first series of experiments, the type A and B
samples were made respectively of PVC and PS. They were subjected five sets of two tribo-charging cycles. The electric potential at the
center of the sample A was measured with the
normal force was increased to 2 N, and five additional sets of two tribo-charging cycles were performed, each followed by a 20-s surface potential decay measurement. Finally, five similar sets of two tribo-charging cycles and surface potential measurement were performed
for two virgin samples A and B, with the 2 N
load (experiment #1.3). The second series of experiments, which are designated as #2.1 and #2.3, were in all respects similar to respectively #1.1 and #1.3, described above, except for the
fact that PS was employed as sample A and
PVC as sample B. The experiments #2.4 and
#2.5 were similar to #2.1, but the normal force was increased to 3 N. The difference between the experiments #2.4 and #2.5, consisted in the
roughness of the PS sample A: 0.02 μm for the
former, 8.5 μm for the latter. A distinct experiment, designated as #3, was performed right after the end of an experiment #1.3. Thus,
the already-charged sample A in PVC, was
subjected to an additional set of two
tribo-charging cycles, then the surface potential decay in its central point was recorded for 3 hours. In the end, the repartition of the potential along the
central longitudinal axis at the surface of an A
-type sample in PVC was measured after six
tribo-charging cycles with a B-type sample in
PS and a load of 2 N (experiment #4.1). The
measurement of the surface potential
distribution was repeated after a second set of six tribo-charging cycles (experiment #4.2). In order to better characterize the surface
distribution of the charge, an A-type PVC
III. RESULTS AND DISCUSSION
The curve in Fig. 4 represents the surface potential continuously recorded at the center of
the sample A (in PVC) for the five
tribo-charging cycles of the experiment #1.1 (sample
B in PS; load 1 N). During the back-and-forth
motion of each tribocharging cycle, the capacitive probe of the electrostatic voltmeter faced also the surface of the insulating belt conveyor (the right-hand limit position of the sample A, in Fig. 2). The positive peaks on the curves correspond to the potential “seen” at the surface of the belt, which is not related to the tribocharging process and are not discussed here. The differences between the positive peak heights are due to the fact that the
better control the applied load and the position of sample B. The experiment #1.3 confirmed the fact that the sample attains quite easily a saturation potential (Fig. 6), which seem to be correlated to the force applied to the bodies in sliding contact. However, the derivation of a statistically significant correlation between this force and the value of the maximum measured potential would require more experiments carried out with an experimental bench provided with means to control the ambient conditions (temperature and relative humidity), to adjust the load and to guarantee its uniform distribution on the contact area between the two surfaces. The observations made in the second
series of experiments (sample Ain PS and
sample B in PVC) are similar to those described
above. The progressive increase of the potential with the number of tribo-charging cycles for two loads (1 N and 2 N) is displayed in Fig. 7, for two typical experiments #2.1 and #2.3. The saturation occurred after eight tribo-charging cycles, at values that are not statistically significant different than those in experiments #1. The load change from 1 to 2 N has less effect on the PS samples in Fig. 7, than on the PVC samples in Fig. 5, as they get more easily close to saturation.
The effect of surface roughness on the tribocharging process can be examined in Fig. 8,
distribution of the electric charges in an area defined by that point. Represented in Fig. 9 are two typical curves obtained in experiment #4, after respectively 6 and 12 tribo-charging cycles. Quite surprisingly, the potential recorded in the latter case is not higher in every point of the samples. The pattern of surface potential distribution varies from one experiment to the other, which may be explained by the differences in the intrinsic structure of the polymers, and the mechanical imperfections of the experimental device. However, in all cases, the potential recorded in the peripheral zones of the samples was higher (in absolute values) that that measured in the central zone.
The 2D plot obtained for the 3 N loaded A-type
PVC sample in experiment #4.3 can be examined in Fig. 10. It confirms the above observations. The increased potential measured in the peripheral zones of the samples is most probably due to the slight machining imperfections of the edges of sample B, which imply increased local roughness and pressure, and hence higher local values of the friction coefficient between the two samples in those peripheral zones, where rubbing changes the direction.
The experiments described in this paper concern the tribocharging of only one pair of polymers:
PS and PVC. Therefore, further studies, with other materials (polycarbonate, polyacetate, …), should be performed in order to confirm the following conclusions:
(1) The surface potential attains a saturation value after a limited number of tribo-charging cycles. This value is higher when the force exerted on the surface of contact between the two polymers is higher, most probably due to the thermal activation related to the energy dissipated in the friction process, but also to the possible transfer of material between the bodies in contact.
(2) The charges transferred in the tribo-charging process at higher load are quite stable, the surface potential decay being very slow.
(3) The distribution of the charges at the surface of the samples is non-uniform, with higher values recorder closer to the edges of the samples. The roughness of the edges of sample B may explain the higher local values of the friction coefficient and of the contact pressure between the two samples in that zones, where rubbing changes the direction. This non-uniformity is likely to affect the lubrication conditions of sliding contacts.
sliding conformal contacts between polymeric materials. The experimental bench should be provided with more accurate means to control the position of the sample and the environmental conditions (temperature and relative humidity of ambient air), as well as with auxiliary devices to adjust the load and to guarantee its uniform distribution on the contact area between the two surfaces.
(5) A larger number of experiments should be
performed, using such an improved
experimental bench, in order to make possible the statistical evaluation of the effects of the various factors that might affect the charging state of the polymers. Of particular interest would be the investigation of the effects of ambient temperature and relative humidity on the distribution and on the decay of the potential at the surface of the samples.
 D. W. Van Krevelen, Properties of
Polymers. Amsterdam: Elsevier, 1990.
 Z. Rymuza, Tribology of Polymers, Arch.
Civil. & Mech. Eng., vol. 7, pp. 177-184, 2007.  S. Bai, P. Huang, Y. Meng, and S. Wen, “Modeling and Analysis of interfacial
electro-kinetic effects on thin film lubrication,” Tribol.
Int., vol. 39, pp. 1405-1412, 2006
 J. B. Gajewski and M. J. Glogowski, “Tribocharging in a rotating shaft-oil-seal
system and the effect of an external electric
field,” J. Electrostat., vol. 63, pp. 1049-1055,
 J. B. Gajewski and M. J. Glogowski, “Influence of additives blended with motor base oils on the braking torque under an auxiliary external DC electric field,” J. Electrostat., vol. 71, pp. 1100-1103, 2013.
 W.R. Harper, Contact and Frictional
Electrification, London, UK: Oxford University Press, 1967, reprinted by Morgan Hill, CA: Laplacian Press, 1998.
 G.S.P. Castle, “Contact charging between insulators,” J. Electrostat., vol. 40&41, pp. 13-18, 1997.
 J. Chubb, “The assessment of materials by tribo and corona charging and charge decay
measurements,” The Institute of Physics
Conference Series No. 163, Bristo, UK: Institute of Physics Publishing, 1999, pp. 329–333.  W. D. Greason, “Inversigation of a test
methodology for triboelectrification,” J.
Electrostat., vol. 49, pp. 245-256, 2000.
 R. G. Horn and D. T. Smith, “Contact electrification and adhesion between dissimilar materials,” Science, vol. 256, pp. 362-364, 1992.
 E. Nemeth, V. Albrecht, G. Schubert, and F. Simon, “Polymer tribo-electric charging:
properties and relative humidity,” J. Electrostat., vol. 58, pp. 3-16, 2003.
 M. D. Hogue, C. R. Buhler, C. I. Calle, T. Matsuyama, W. Luo, and E.E. Groop, “Insulator-insulator contact charging and its
relationship with atmospheric pressure,” J.
Electrostat., vol. 61, pp. 259-268, 2004.
 K. Hiratsuka and K. Hosotani, “Effects of friction type and humidity on triboelectrification and triboluminiscence among eight kind of
polymers,” Tribol.Int., vol. 55, pp. 87-99, 2012.
 K. Nakayama, “Tribocharging and friction
in insulators in ambient air,” Wear, vol. 194, pp.
 C. Guerret-Piecourt, S. Bec, and D. Treheux, “Electrical charges and tribology of
insulating materials,” ComptesRendus de
l’Académie des Sciences – Series IV – Physics, vol. 2, pp. 761-774, 2001.
 B. Kchaou, C. Turki, M. Salvia, Z. Fakhfakh, and D. Treheux, “Dielectric and friction behavior of unidirectional glass fiber
reinforced epoxy (GFRE),” Wear, vol. 265, pp.
 L. Jian, L. Ning, S. Yang, J. Wang, and M. Hua, “Triboelectrification electrostatic potential of MC Nylon 6 under point contact dry sliding,”
Tribol. Lett., vol. 36, pp. 199-208, 2009.
 T. A. L. Burgo, C.A. Rezende, S. Bertazzo, A. Galembeck, and F. Galembeck, “Electric
potential decay on polyethylene: role of atmospheric water on electric charge build–up
and dissipation,” J. Electrostat., vol. 69, pp.
 T. A. L. Burgo, C. A. Silva, L. B. S. Balestin, and F. Galembeck, “Friction
coefficient dependence on electrostatic
tribocharging,” Scientific Reports, vol. 3, 2013,
 A. F. Diaz, and R. M. Felix-Navarro, “A semi-quantitative tribo-electric series for polymeric materials: the influence of chemical
structure and properties,” J. Electrostat., vol. 62,
pp. 277–290, 2004.
 K. L. Johnson, Contact Mechanics.
Cambridge: Cambridge Univ. Press, 1985, pp. 107-196.
 Y.-P. Chang, J.-P.Yur, N.-H.Chou, and H.-M. Chub, “Tribo-electrification mechanisms for self-mated carbon steels in dry severe wear
process.Wear, vol. 260, pp. 1209–1216, 2006
 B. Kchaoua, C. Turki, M. Salvia, Z. Fakhfakh, and D. Tréheux, “Dielectric and friction behaviour of unidirectional glass fibre
reinforced epoxy (GFRE)”, Wear, vol. 265, pp.
conveyers,” J. Electrostat., vol. 40/41, pp. 277– 282, 1997.
 C. Dragan, M. Bilici, S. Das, A. Samuila, and L. Dascalescu, “Tribocharging of insulating powders in annular ducts of pneumatic devices,”
IEEE Trans. Ind. Appl., vol. 46, pp. 1238-1243, 2010.
Receivedthe B.Tech degree in Electronics& Communication Engineering fromSreeDattha Institute of Engineering & Science 2013 from JNTU, Hyderabad, Telangana, Indiaand She
completed M.Tech in Electronics&
Communication Engineering as specialization in the Department ofElectronics& Communication Engineering in 2017 from JNTU Hyderabad Teangana India.She iscurrently an Assistant
Professor with the
Engineering.at SLC CollegeJntu University, Hyderabad, Telangana India. Her research interests include in the area of RF and Microwave Engineering andOptical networks.
Ramavath Shankar Naik
received the B.Tech degree in Electrical
Engineering from Vignan’s Engineering
College, Vadlamudi, Guntur, India, in 2006. He Completed M.E in Electrical Engineering with Power systemAutomation as specialization in the Department of Electrical Engineering, Andhra University College of Engineering (Autonomous), Visakhapatnam, He is currently an Assistant Professor with the Department of Electrical &Electronic Engineering at SLC College Jntu University, Hyderabad, Telangana, India. His area of interest lies in Power system operation and control.and optimal operation of power systems, and FACTS.